Abstract
Magnons and phonons are fundamental quasiparticles in a solid and can be coupled together to form a hybrid quasiparticle. However, detailed experimental studies on the underlying Hamiltonian of this particle are rare for actual materials. Moreover, the anharmonicity of such magnetoelastic excitations remains largely unexplored, although it is essential for a proper understanding of their diverse thermodynamic behaviour and intrinsic zerotemperature decay. Here we show that in noncollinear antiferromagnets, a strong magnon–phonon coupling can significantly enhance the anharmonicity, resulting in the creation of magnetoelastic excitations and their spontaneous decay. By measuring the spin waves over the full Brillouin zone and carrying out anharmonic spin wave calculations using a Hamiltonian with an explicit magnon–phonon coupling, we have identified a hybrid magnetoelastic mode in (Y,Lu)MnO_{3} and quantified its decay rate and the exchangestriction coupling term required to produce it.
Similar content being viewed by others
Introduction
Spin and lattice constitute two of the four fundamental degrees of freedom in the solid: the other two are charge and orbital. In linearized models that account for many current understandings of the solid, excitations of spin and lattice, magnon of spin waves and phonon of lattice vibrations, are two principal examples of such quasiparticles^{1}. Although there have been some experimental observations of crosscoupling between magnon and phonon, it is rather rare to actually observe and, more importantly, quantify the magnon–phonon coupling for real materials^{2,3}. Nevertheless, it is essential for a proper understanding of their diverse thermodynamic behaviour and intrinsic zerotemperature decay^{4}. Furthermore, it is generally believed that the magnon–phonon coupling is important for materials such as multiferroic compounds, geometrically frustrated systems, spinPeierls systems and Invar materials, to name only a few^{5,6,7,8}.
Quasiparticles like magnon and phonon, the cornerstone of modern condensed matter physics, are fundamentally the byproducts of linearized theories that ignore all the higherorder terms than quadratic terms and neglect any conceivable interaction among the quasiparticles themselves. As such, they are considered to be stable, except for very few exceptions. For example, for classical spin systems without strong quantum fluctuations, magnon breakdown is thought to be unlikely for most of purposes. Therefore, observing and understanding how the otherwise stable quasiparticles break down in these unusual cases are the central theme of condensed matter physics.
One route leading to the breakdown of magnon and phonon is the cubic anharmonicities. Despite the general belief that this nonlinear magnon(magnon) interaction is rather weak in real materials, recent insights gained mainly through theoretical studies suggest that things should be drastically different for certain cases, namely for noncollinear antiferromagnetic structures^{4}. Unlike collinear magnetic structures that forbid the cubic anharmonicities, it was shown that such interaction is in principle allowed for noncollinear magnetic structures, such as the canonical 120° spin pattern in a twodimensional (2D) triangular lattice. There have since been several experimental reports^{9,10} supporting these theoretical postulates. Nevertheless, the full details of the nonlinear interaction still need to be worked out, especially from experiments. We should also point out that this noncollinear magnetic order, in principle, allows a hitherto forbidden magnon–phonon coupling that has been less recognized among the community: the firstorder variation of the exchange energy with respect to transverse spin fluctuations is nonzero for a noncollinear magnetic order^{11}. As the O(3) symmetry is completely broken in the noncollinear ordered ground state of spins, coupling to phonons necessarily generates a coupling in which a magnon can convert directly into a phonon and vice versa. This is in contrast to the spin–lattice coupling in more conventional, collinear magnets, where the coupling usually respects the parity, which necessarily conserves the number of magnons or allows creation (annihilation) of them only in pairs^{12}.
Here we report the direct observation of the magnon–phonon coupling and the spontaneous decay of magnetoelastic excitations in the triangular antiferromagnets (Y,Lu)MnO_{3}. The full magnetic excitation spectra measured by inelastic neutronscattering experiments show clear deviations from the linear spin wave theory without the magnon–phonon coupling: an additional mode at high energies and the downward shift of the bottom mode at the Brillouin zone boundary. This is the most direct and stark evidence of the linear coupling of magnons and phonons, which, in turn, leads to enhancement of the anharmonic effects. We demonstrate that these experimental anomalies can only be fully resolved by incorporating the magnon–phonon coupling and carrying out the nonlinear spin wave analysis. We further reveal that the magnetoelastic excitation leads to significant broadening of the magnon spectra at the zone boundaries, originating from the decay of the magnetoelastic excitations into the twomagnon continuum.
Results
Failure of standard spin waves calculation
Hexagonal rareearth manganite RMnO_{3} represents a good model system for geometrical frustration on a 2D triangular lattice: the nearestneighbour antiferromagnetic interaction between S=2 (Mn^{3+}) spins dominate, whereas the interlayer interaction is relatively weak^{13,14}. We should note that it also exhibits a very large spin–lattice coupling when it becomes magnetically ordered^{5}. In a more recent work, we reported experimental evidence for a spontaneous magnon decay and a remarkably large spatial anisotropy for Mn^{3+} ions in the exchange interactions for LuMnO_{3}. This was attributed to a structural distortion in which groups of three Mn atoms become more closely bound^{9}, such that the intratrimer J_{1} exchange constants may differ from the intertrimer J_{2} (see Fig. 1). Similar interpretations were shared by other groups too^{15,16}. However, we should note that the large J_{1}/J_{2} ratio of 6.4 obtained from fitting the data is inconsistent with the value of 1.15, obtained from firstprinciples calculations^{17} that used the experimental atomic positions as reported by neutron diffraction^{5}. This realization prompted us to handle both magnon and phonon, as well as their crosscoupling on an equal footing and to go beyond the linear spin wave analysis.
Figure 1 shows the spin waves measured at the MAPS beamline of the ISIS facility together with the theoretical dispersion relation calculated from the spin Hamiltonian by a linear spin wave theory using the following parameters (see Supplementary Note 2): for YMnO_{3}: J_{1}=4, J_{2}=1.8, D_{1}=0.28, D_{2}=−0.02 meV; for Y_{0.5}Lu_{0.5}MnO_{3}: J_{1}=12.5, J_{2}=0.97, D_{1}=0.18, D_{2}=−0.018 meV; for LuMnO_{3}: J_{1}=9, J_{2}=1.4, D_{1}=0.28, D_{2}=−0.02 meV. Despite the apparent success of the linear spin wave calculations, there lies a critical failure: first, the downward curvature along the AB direction and, second, the additional peaks at ∼19 meV indicated by a red box in Fig. 1c–e. However, most importantly, here we have to use an unphysically large J_{1}/J_{2} ratio, to explain the additional highenergy peaks. Apart from the large J_{1}/J_{2} ratio, this analysis of the linear spin waves has another drawback: which is that the calculated dynamical structure factor using the linear spin wave theory as shown in Fig. 1f–h always produces stronger intensity at the top mode of the spin waves than at the middle one, in marked contrast with the experimental data.
This discrepancy requires us to adopt a radically different approach to explain the measured full spin waves and go beyond the standard linear spin wave theory. One clue for how to address this problem can be taken from the physical properties: for example, our earlier neutron diffraction data revealed a giant spin–lattice coupling for (Y,Lu)MnO_{3} (ref. 5). This observation was subsequently corroborated by independent measurements on rareearth hexagonal RMnO_{3} (refs 18, 19, 20, 21, 22, 23, 24, 25). More importantly, ultrasound measurements on YMnO_{3} found marked softening in C_{11} and C_{66}, supporting our view that there is a strong inplane deformation below T_{N}^{26}. This observation naturally indicates the importance of magnon and inplane phonon coupling. This conclusion is also backed up by theoretical calculations^{17,27}.
Calculation of magnetoelastic excitations
Following this idea of a large spin–lattice coupling in RMnO_{3}, we took a firstprinciples approach to the magnon–phonon coupling. First, we construct the following full model Hamiltonian, which couples the inplane manganese vibrations directly to the spin system:
where denotes the unit vector connecting the ith manganese atom and the neighbouring oxygen atoms between the ith and jth manganese atoms as shown in Supplementary Fig. 2, is the exchange striction, , which is naturally made into a dimensionless exchange–striction constant ^{28}, and d is the Mn–O bond length at the equilibrium. Therefore, our Hamiltonian takes into account the modulations of the Mn–O bond length as a function of Mn displacements.
Before going into detailed discussion, we would like to make a general remark on the related issue. In cases when the spin rotational symmetry is broken completely in the ground state, that is, when the spin structure is noncollinear, the Heisenberg term of the Hamiltonian provides a coupling of the transverse and longitudinal modes on neighbouring sites. That is, in terms of the local sitedependent preferred spin direction of the ordered state, the coupling terms take the form of the type and so on. In the magnon language, they are quantized into the ‘odd’ terms, producing linear and cubic (a^{†}aa and so on) contributions. In equilibrium, the linear magnon term must vanish, leaving the anharmonic cubic magnon coupling to be the sole outcome, which is important for magnon decays. However, in the presence of coupling to phonons, the linear terms is ‘activated’, as the local atomic displacements (u_{i}) violate the equilibrium conditions locally, hence the ‘direct’ coupling of magnons and phonons.
To calculate the full dispersions of all 90 phonon modes for the unit cell with six formula units, we used a firstprinciples density functional theory (DFT). We show the full phonon dispersion curves for the three compounds as dashed lines in Fig. 2. We note that the calculated phonon density of states (DOS) is in good agreement with the phonon spectra we measured using powder YMnO_{3} and LuMnO_{3} at the AMATERAS beamline of JPARC (see Supplementary Fig. 1). We then calculated the dynamical spin structure factor within the linear approximation by using the full Hamiltonian above with the explicit magnon–phonon coupling: we used the dimensionless exchange–striction coefficients of α∼16–20.
The exchange–striction constant can also be estimated by using the pressure dependence of the crystal structure and the antiferromagnetic transition reported for YMnO_{3} (refs 29, 30). Using the experimental data reported in refs 9, 10, we came to an estimate of the dimensionless exchange striction α of 14 with the following formula: . Here, d is average Mn–O bond length, which is approximately onethird of lattice constant a. The experimental parameters used in our estimate are K GPa^{−1} (ref. 29) and Å GPa^{−1} (ref. 30). Below we point out that our own data for the magnon excitation spectrum imply the value of the magnetostriction of the same order. This should be contrasted with the cuprates family, where estimates for an equivalent quantity are substantially smaller, α∼2–7(refs 31, 32).
By comparing with the experimental data, we obtained the best fitting results with the following sets of the parameters: J_{1}=J_{2}=2.5 meV, D_{1}=0.28 meV, D_{2}=−0.02 meV and α=16 for YMnO_{3}; J_{1}=J_{2}=2.7 meV, D_{1}=0.28 meV, D_{2}=−0.02 meV and α=20 for Y_{0.5}Lu_{0.5}MnO_{3}; and J_{1}=J_{2}=3 meV, D_{1}=0.28 meV, D_{2}=−0.02 meV and α=16 for LuMnO_{3} (see Supplementary Table 1). We note that according to the DFT calculations^{17} the relative difference between J_{1} and J_{2} is theoretically about 10–20% at maximum. Therefore, we judge that this choice of J_{1}=J_{2} in our analysis is good enough to capture the essential underlying physics of (Y,Lu)MnO_{3}, which is the magnon–phonon coupling.
The results shown as colour contour plot in Fig. 2 reproduce the overall features of the observed spectra of the experimental data in Fig. 1. It clearly shows that the highenergy signals located at 18∼20 meV come from a direct coupling between the magnon and the optical phonons, that is, a magnetoelastic mode. The intensity of this high energy magnetophonon modes becomes stronger for Luenriched compounds due to the larger Mn phonon DOS at this energy for the Luenriched compounds, consistent with the experimental results shown in Fig. 1. This conclusion on the relevance of the magnon–phonon coupling for RMnO_{3} is also supported by the fact that our calculated spin waves successfully explains the downward curvature of the bottom magnon branch along the AB direction. In fact, an estimate of the exchange striction from the splitting of the highenergy hybrid modes in Fig. 2 yields the values in the same range, α∼10–20 (see Supplementary Note 3). We also note that our polarized neutronscattering data are in good agreement with our calculations (see Supplementary Fig. 4 and Supplementary Note 4).
Spontaneous decay of the hybrid mode
In addition to the magnon–phonon hybridization, noncollinear spin structures allow three magnon interactions as discussed above, which can lead to spontaneous magnon decay into two magnon states when the kinematic conditions are satisfied. The magnetoelastic excitations have, by definition, both magnon and phonon characters. Therefore, the above mechanism can also lead to the decay of magnetoelastic excitations inside the two quasiparticles continuum of magnon. Indeed, we observe significant broadening of the top mode in LuMnO_{3} near the B and D points as shown in Fig. 3 and Supplementary Fig. 3: less strong broadening has been seen for other two compounds.
To calculate the decay rate directly and compare it with the experimental data, we simplify the problem by assuming a dispersionless optical phonon mode at ∼20 meV, where the strongest coupling has been observed in our data. Next, our model Hamiltonian reads as follows:
First, we calculate the dynamical spin structure factor by using a standard method. As shown in Fig. 3a, despite the simplification, the calculation results reproduce well the experimental intensity along the C–B–D direction. For the calculations, we used the following set of the parameters: for YMnO_{3}: J=2.7 meV, γ=0.93, ħω_{0}=17.5 meV, α=7.2; for LuMnO_{3}: J=3.2 meV, γ=0.93, ħω_{0}=19.5 meV, α=8. Next, the decay rate of the highenergy mode was calculated using an anharmonic spin wave theory within the 1/S approximation. The calculated results summarized in Fig. 3 also show the significant linewidth broadening for the top mode near the B and D points only for LuMnO_{3}, consistent with the experimental results.
The reason for this is that in LuMnO_{3}, the combination of the higher energies of the magnon and magnetoelastic modes means that more decay channels, including two quasiparticle emission, are kinematically allowed. The different decay channels have different boundaries in the reciprocal space, which also corresponds to logarithmic singularities in the decay rate^{33}, and the largest broadening is observed at momentum transfers where the singlequasiparticle dispersion crosses these boundaries, such as at the B point. In the case of YMnO_{3}, no such crossing occurs; thus, there are fewer decay channels available explaining why the observed linewidths remain narrow. Here we should stress that the singlemagnon branches do not cross the line of singularities, whereas the magnetoelastic mode does; thus, a pure magnon decay is forbidden in this case. Similarly, the intrinsic decay rate of phonons is usually small due to a weak cubic anharmonicity. Thus, the strong hybridization of magnons and phonons provides a new mechanism to enhancing the magnon decays.
Discussion
Our studies using an exchangestriction model indicates that the deviations from the linear spin wave theory must be a common feature for other triangular antiferromagnets with a noncollinear magnetic order. Looking beyond the 2D triangular antiferromagnets, we believe that the idea of magnon–phonon coupling can also be important in the studies of a wide variety of the 3d transitionmetal magnetic compounds. For example, similar analysis might shed a light on the investigation of spin phonon coupling mechanism and anharmonic effects in many other important noncollinear magnets that exhibit a rather large spin–lattice coupling, such as spinel^{34} and invar materials^{35}, which should be dominated by the exchange–striction as discussed in ref. 36. This is in contrast to the previous studies on magnon–phonon coupling focusing on materials with strong spin–orbit coupling such as rareearth elements^{37}.
To summarize, we mapped out the spin waves and phonon excitations of (Y,Lu)MnO_{3} over the Brillouin zone. By carrying out the spin wave calculations using the full Hamiltonian with both magnons and phonons on an equal footing and their coupling, we have not only demonstrated in our inelastic neutronscattering data a clear sign of magnon–phonon coupling, but also have quantified the coupling strength directly. Our work provides the rare experimental test and quantification of magnon–phonon coupling in real materials and opens a new window of opportunities in other materials such as 2D triangular lattice and other frustrated systems, where such couplings, hitherto hidden, have been long suspected.
Methods
Sample preparation
We synthesized powder samples using a solidstate reaction method following the recipe as described in the literature^{38}. We then grew single crystals of Y_{1−x}Lu_{x}MnO_{3} (with typical size of 5 × 5 × 40 mm^{3}) by using a commercial optical floating zone furnace (Crystal Systems, Japan). Our subsequent powder and single crystal XRD confirmed that all our samples are prepared in high quality. We also measured the bulk properties (susceptibility and heat capacity) of all the samples to further confirm the quality by using a commercial setup (MPMS5XL and PPMS9, Quantum Design USA).
Inelastic neutron scattering
Inelastic neutronscattering experiments have been performed on single crystal samples using the MAPS timeofflight spectrometer at ISIS, UK, and a triple axes spectrometer with polarization analysis at Chalk River, Canada. In the timeofflight experiments, incident energies were chosen at 40 meV for LuMnO_{3}, 35 meV for Y_{0.5}Lu_{0.5}MnO_{3} and 30 meV for YMnO_{3} to adjust to the slight variations in the energy scales for each samples. The chopper frequency has been set to 250 Hz, which gave us a full width at half maximum energy resolution of 0.43∼1.36 meV depending on the energy transfer. The measurements have been performed at 4 K for YMnO_{3} and Y_{0.5}Lu_{0.5}MnO_{3}, and 13 K for LuMnO_{3}. We used the Horace programme for our data analysis^{39}. In the triple axes spectrometer experiments, spinpolarized neutrons have been produced by using vertical focusing Heusler monochromator and analyser with the final energy fixed at 13.7 meV. To measure phonon DOS, inelastic neutronscattering experiments have also been performed on the powder samples with the incident energy of 42 meV using the AMATERAS beamline at JPARC, Japan.
Theoretical calculations
We carried out firstprinciples calculations of phonon using a DFT+U method with U=4 eV. We used the PHONOPY code based on the force constant method^{40}. In addition, the force constants were constructed by means of a supercell approach based on the density functional perturbation theory^{41}, implemented in the VASP code^{42}. Detailed discussion is given in the Supplementary Note 1.
For the spin waves calculations, we used a rotating framework with the direction of easy axis anisotropy being rotated from parallel to perpendicular to the crystallographic axes. To make our calculations simpler and transparent, we ignored the interlayer exchange coupling as it is known to be more than 100 times smaller than the inplane coupling^{9,14}. Using this approximation, we can have the following minimal Hamiltonian:
where J_{1} and J_{2} represent intra and intertrimer exchange constants and D_{1} and D_{2} are two magnetic anisotropies. We then calculated the spin wave dispersion using the standard linear spin wave theory^{43}. We give detailed description of our spin wave calculations for the full Hamiltonian with the magnon and phonon coupling and the magnon–magnon nonlinear interaction in the Supplementary Notes 2 and 3.
Data availability
All relevant data that support the findings of this study are available from the corresponding author on request.
Additional information
How to cite this article: Oh, J. et al. Spontaneous decays of magnetoelastic excitations in noncollinear antiferromagnet (Y,Lu)MnO_{3}. Nat. Commun. 7, 13146 doi: 10.1038/ncomms13146 (2016).
References
Landau, L. D. The theory of a Fermi liquid. Sov. Phys. JETP 3, 920–925 (1957).
Pimenov, A. et al. Possible evidence for electromagnons in multiferroic manganites. Nat. Phys. 2, 97–100 (2006).
Ogawa, N. et al. Photodrive of magnetic bubbles via magnetoelastic waves. Proc. Natl Acad. Sci. USA 112, 8977–8981 (2015).
Zhitomirsky, M. E. & Chernyshev, A. L. Colloquium: spontaneous magnon decays. Rev. Mod. Phys. 85, 219–242 (2013).
Lee, S. et al. Giant magnetoelastic coupling in multiferroic hexagonal manganites. Nature 451, 805–809 (2008).
Buschow K. H. J. (ed.) Handbook of Magnetic Materials Vol.13, Elsevier, Amsterdam (2001).
Hase, M., Terasaki, I. & Uchinokura, K. Observation of the spinPeierls transition in linear Cu^{2+} (spin1/2) chains in an inorganic compound CuGeO3 . Phys. Rev. Lett. 70, 3651–3654 (1993).
Kim, D. J. The electronphonon interaction and itinerant electron magnetism. Phys. Rep. 171, 129–229 (1988).
Oh, J. et al. Magnon breakdown in a two dimensional triangular lattice Heisenberg antiferromagnet of multiferroic LuMnO3 . Phys. Rev. Lett. 111, 257202 (2013).
Toth, S. et al. Magnetic soft modes in the distorted triangular antiferromagnet αCaCr2O4 . Phys. Rev. Lett. 109, 127203 (2012).
Kim, J. H. & Han, J. H. Coupling of phonons and spin waves in a triangular antiferromagnet. Phys. Rev. B 76, 054431 (2007).
Dixon, G. S. Lattice thermal conductivity of antiferromagnetic insulators. Phys. Rev. B 21, 2851–2864 (1980).
Sim, H., Oh, J., Jeong, J., Le, M. D. & Park, J.G. Hexagonal RMnO3: a model system for 2D triangular lattice antiferromagnets. Acta. Cryst. B 72, 3–19 (2016).
Fabrèges, X. et al. Spinlattice coupling, frustration, and magnetic order in multiferroic RMnO3 . Phys. Rev. Lett. 103, 067204 (2009).
Sato, T. J. et al. Unconventional spin fluctuations in the hexagonal antiferromagnet YMnO3 . Phys. Rev. B 68, 014432 (2003).
Lewtas, H. J., Boothroyd, A. T., Rotter, M. & Prabhakaran, D. Magnetic excitations in multiferroic LuMnO3 studied by inelastic neutron scattering. Phys. Rev. B 82, 184420 (2010).
Solovyev, I. V., Valentyuk, M. V. & Mazurenko, V. V. Magnetic structure of hexagonal YMnO3 and LuMnO3 from a microscopic point of view. Phys. Rev. B 86, 054407 (2012).
Litvinchuk, A. P., Iliev, M. N., Popov, V. N. & Gospodinov, M. M. Raman and infraredactive phonons in hexagonal HoMnO3 single crystals: magnetic ordering effects. J. Phys. Condens. Matter 16, 809–819 (2004).
Souchkov, A. B. et al. Exchange interaction effects on the optical properties of LuMnO3 . Phys. Rev. Lett. 91, 027203 (2003).
Dela Cruz, C. et al. Strong spinlattice coupling in multiferroic HoMnO3: thermal expansion anomalies and pressure effect. Phys. Rev. B 71, 060407R (2005).
Park, J. et al. Doping dependence of spinlattice coupling and twodimensional ordering in multiferroic hexagonal Y1−xLuxMnO3 (0<x<1). Phys. Rev. B 82, 054428 (2010).
Chatterji, T., Ouladdiaf, B., Henry, P. F. & Bhattacharya, D. Magnetoelastic effects in multiferroic YMnO3 . J. Phys. Condens. Matter 24, 336003 (2012).
Petit, S. et al. Spin phonon coupling in hexagonal multiferroic YMnO3 . Phys. Rev. Lett. 99, 266604 (2007).
Sharma, P. A. et al. Thermal conductivity of geometrically frustrated, ferroelectric YMnO3: extraordinary spinphonon interactions. Phys. Rev. Lett. 93, 177202 (2004).
Pailhès, S. et al. Hybrid Goldstone modes in multiferroic YMnO3 studied by polarized inelastic neutron scattering. Phys. Rev. B 79, 134409 (2009).
Poirier, M. & Laliberté, F. Magnetoelastic coupling in hexagonal multiferroic YMnO3 using ultrasound measurements. Phys. Rev. B 76, 174426 (2007).
Varigon, J., Petit, S., Gell´e, A. & Lepetit, M. B. An ab initio study of magnetoelectric coupling of YMnO3 . J. Phys. Condens. Matter 25, 496004 (2013).
Bramwell, S. T. Temperature dependence of the isotropic exchange constant. J. Phys. Condens. Matter 2, 7527–7536 (1990).
Lancaster, T. et al. Magnetism in geometrically frustrated YMnO3 under hydrostatic pressure studied with muon spin relaxation. Phys. Rev. Lett. 98, 197203 (2007).
Kozlenko, D. P. et al. Highpressure effect on the crystal and magnetic structures of the frustrated antiferromagnet YMnO3 . JETP Lett. 82, 212–216 (2005).
Häfliger, P. S. et al. Quantum and thermal ionic motion, oxygen isotope effect, and superexchange distribution in La2CuO4 . Phys. Rev. B 89, 085113 (2014).
Chernyshev, A. L. & Brenig, W. Thermal conductivity in largeJ twodimensional antiferromagnets: role of phonon scattering. Phys. Rev. B 92, 054409 (2015).
Chernyshev, A. L. & Zhitomirsky, M. E. Spin waves in a triangular lattice antiferromagnet: decays, spectrum renormalization, and singularities. Phys. Rev. B 79, 144416 (2009).
Ji, S. et al. Spinlattice order in frustrated ZnCr2O4 . Phys. Rev. Lett. 103, 037201 (2009).
Schilfgaarde, M. V., Abrikosov, I. A. & Johansson, B. Origin of the Invar effect in ironnikel alloys. Nature 400, 46–49 (1999).
Tchernyshyov, O., Moessner, R. & Sondhi, S. L. Order by distortion and string modes in pyrochlore antiferromagnets. Phys. Rev. Lett. 88, 067203 (2002).
Jensen, J. & Houmann, J. G. Spin waves in terbium. II. Magnonphonon interaction. Phys. Rev. B. 12, 320–331 (1975).
Chandra Sekhar, M., Lee, S., Choi, G., Lee, C. & Park, J.G. Doping effects of hexagonal manganites Er1−xYxMnO3 with triangular spin structure. Phys. Rev. B 72, 014402 (2005).
Ewings, R. A. et al. HORACE: software for the analysis of data from single crystal spectroscopy experiments at timeofflight neutron instruments. Nucl. Instrum. Meth. A 834, 132–142 (2016).
Parlinski, K., Li, Z. Q. & Kawazoe, Y. Firstprinciples determination of the soft mode in cubic ZrO2 . Phys. Rev. Lett. 78, 4063–4066 (1997).
Baroni, S., De Gironcoli, S., Dal Corso, A. & Giannozzi, P. Phonons and related crystal properties from densityfunctional perturbation theory. Rev. Mod. Phys. 73, 515–562 (2001).
Kresse, G. & Furthműller, J. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Phys. Rev. B 54, 11169–11186 (1996).
White, R. M. et al. Diagonalization of the antiferromagnetic magnonphonon interaction. Phys. Rev. 139, A450–A454 (1965).
Acknowledgements
We thank Kisoo Park and W.J.L. Buyers for useful discussions. The work at the IBS CCES was supported by the research programme of Institute for Basic Science (IBSR009G1). Experiment at JPARC was carried out through the proposal number (2011B0064). The work of ALC was supported by the U.S. DOE, Office of Science, Basic Energy Sciences under Award Number DEFG0204ER46174. The work at Rutgers University was supported by the DOE under Grant Number DOE: DEFG0207ER46382.
Author information
Authors and Affiliations
Contributions
J.G.P. conceived and supervised the project. H.S., Y.Y., H.E. and S.W.C. grew the single crystals and H.S. carried out bulk characterization. J.O., M.D.L., J.J., T.G.P., H.W., K.N., S.O.K., Z.Y. and J.G.P. were involved in the neutron scattering experiments. H.H.N. carried out firstprinciples phonon calculation and J.O. made all the spinwave calculations under the guidance of J.G.P. and A.L.C. J.G.P., J.O. and A.L.C. wrote the paper after discussion with all the authors.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 14, Supplementary Table 1, Supplementary Notes 14 and Supplementary References (PDF 641 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Oh, J., Le, M., Nahm, HH. et al. Spontaneous decays of magnetoelastic excitations in noncollinear antiferromagnet (Y,Lu)MnO_{3}. Nat Commun 7, 13146 (2016). https://doi.org/10.1038/ncomms13146
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/ncomms13146
This article is cited by

Field control of quasiparticle decay in a quantum antiferromagnet
Nature Communications (2024)

Thermal Hall effects due to topological spin fluctuations in YMnO3
Nature Communications (2024)

Instabilities of heavy magnons in an anisotropic magnet
Nature Communications (2023)

Anisotropic magnon damping by zerotemperature quantum fluctuations in ferromagnetic CrGeTe3
Nature Communications (2022)

Angularly quantized spin rotations in hexagonal LuMnO3
Scientific Reports (2022)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.